OPEN SUBJECT AREAS: MECHANICAL ENGINEERING MATERIALS SCIENCE
Received 15 August 2013 Accepted 8 October 2013 Published 29 October 2013
Correspondence and requests for materials should be addressed to
Airtight metallic sealing at room temperature under small mechanical pressure Stephen P. Stagon1 & Hanchen Huang1,2 1
Department of Mechanical Engineering, University of Connecticut, Storrs, CT 06269, USA, 2Department of Mechanical and Industrial Engineering, Northeastern University, Boston, MA 02115, USA.
Metallic seals can be resistant to air leakage, resistant to degradation under heat, and capable of carrying mechanical loads. Various technologies – such as organic solar cells and organic light emitting diodes – need, at least benefit from, such metallic seals. However, these technologies involve polymeric materials and can tolerate neither the high-temperature nor the high-pressure processes of conventional metallic sealing. Recent progress in nanorod growth opens the door to metallic sealing for these technologies. Here, we report a process of metallic sealing using small well-separated Ag nanorods; the process is at room temperature, under a small mechanical pressure of 9.0 MPa, and also in ambient. The metallic seals have an air leak rate of 1.1 3 1023 cm3atm/m2/day, and a mechanical shear strength higher than 8.9 MPa. This leak rate meets the requirements of organic solar cells and organic light emitting diodes.
H.C.H. ([email protected]
o begin, we first use organic solar cells (OSCs) as an example to demonstrate the challenges of sealing and identify the need of metallic sealing at room temperature, under small mechanical pressure, and preferably in ambient environment1–7. As shown in Figure 1, an organic semiconductor core of an OSC is encapsulated to avoid exposure to air, particularly oxygen (O2) and water vapor (H2O). The exposure leads to degradation and short lifetime3,4. For flexibility, the encapsulating substrates are usually polymers and have barrier layers on them to minimize the exposure. At the same time, the seals that connect the substrate and the barrier layer must be airtight to minimize the exposure. At present, the seals are polymeric, as shown on the right of Figure 1, and they do not provide sufficient resistance to air leakage, even when new. During operation, the polymer seals degrade and their air leak rate increases even more. As a result, the OSCs have short lifetime, which is one of the main reasons that OSCs are not yet economically competitive4,6. Similarly, organic light emitting diodes (OLEDs) have apparent technological advantage but their wide spread implementation has not been possible due to the exposure and short lifetime6. The metallic seal, shown on the left of Figure 1, can be sufficiently airtight. However, metallic seals are absent in OSCs or OLEDs despite their apparent advantage in air leak resistance. This absence is the result of a major technical challenge – the organic semiconductor core and the polymeric substrates are incompatible with sealing processes at high temperature or high pressure. Recent progress in nanorod growth may open the door for us to address this challenge8. Next, we examine the existing processes of metallic sealing, with particular focus on processing temperature and pressure. Since the sealing temperature must be low to avoid damage to the organic semiconductor core and the polymer substrates, our examination focuses on only those processes at relatively low temperatures. The existing processes fall into three categories. First, the soldering process that has been commonly used in the electronics industry functions much above 60uC with eutectic alloys containing toxic Pb or expensive In9–11. Even without any consideration of toxicity and cost, such alloys that allow soldering around 60uC have low mechanical strength during normal OSC operation, which easily approaches their melting temperature. Further, the soldering process involves corrosive fluxes and the use of vacuum. Second, cold welding of flat surfaces functions at room temperature, but it requires an extremely high compressive load, on the order of about 1 GPa12. However, polymeric substrates may disfigure even at a compressive load that is one order of magnitude lower, about 100 MPa13. Third, sealing with metallic nanoparticles or nanorods takes advantage of fast surface diffusion and occurs at relatively low temperatures14. Using Ag nanoparticles, the sealing process is possible at 160uC through coarsening under a low pressure of about 10 MPa15. The processing temperature, which is too high, cannot be lowered because of the organic capping layer on each nanoparticle that originates from solution synthesis. While it is possible to remove the capping layer with solvents, such solvents are not compatible with
SCIENTIFIC REPORTS | 3 : 3066 | DOI: 10.1038/srep03066
Figure 1 | Need of metallic sealing. Schematic of air, particularly oxygen (O2) and water vapor (H2O), leaking in OSCs.
the organic components of the OSCs and OLEDs16. With notwell-separated Cu nanorods, the sealing process requires a high temperature of 300uC under low pressure in a vacuum or inert environment17. Even without the consideration of the processing cost associated with a non-ambient environment, none of the three categories of seals satisfy the requirements of low temperature and low pressure for OSC and OLED technologies.
Results Here, we propose a metallic sealing process at room temperature under a small mechanical pressure, below 10 MPa, and also in ambient environment. This proposal builds on the growth of small wellseparated metallic nanorods, an ability that has recently become reality8,18. These nanorods do not have capping layers and do not require a high temperature of 160uC to coarsen. Further, we choose Ag for metallic sealing to minimize potential oxidation with only moderate cost. In comparison, Ag costs less than In that is used in eutectic alloys for soldering; and Ag is not volatile as In9–11,19. To ensure good adhesion, we add a metallic film between the Ag nanorods and sealing substrate. Figure 2 schematically illustrates our proposal. Before the sealing process, two substrates carrying the small well-separated Ag nanorods are brought to face each other; Figure 2a. Under a small mechanical pressure, the nanorods from two sides crosslink with each other; Figure 2b. The feasibility of crosslinking is critical in this proposal, and it benefits from the recent realization of small wellseparated nanorods8. Due to the fast diffusion on the surfaces of nanorods, the crosslinked nanorods condense into a film; Figure 2c. The fast surface diffusion is necessary for the proposed sealing process in Figure 2, and it is next verified. Figure 3 shows the morphological change of Ag nanorods during annealing in ambient at constant temperatures; see Supplemental Materials Sections S2 and S3 for details of fabrication, annealing, and characterization of the nanorods. Figure 3a shows the Ag nanorods that are kept at room temperature for about one hour from their synthesis. The bridging between nanorods indicates, non-conclusively, potentially fast surface diffusion even at room temperature, which is nominally 25uC. At 50uC 1/2 4uC, only slightly above room temperature,
the substantial change of morphologies over merely five minutes shows that the surface diffusion is indeed fast; Figure 3b. At 75uC 1/2 6uC, the change of morphologies over five minutes is more dramatic, indicating even faster surface diffusion; Figure 3c. At 100uC 1/2 8uC, the nanorods completely coalesce into a continuous film in five minutes; Figure 3d. This set of annealing results confirms that surface diffusion near room temperature can be fast, and that surface diffusion slightly above room temperature is very fast. Based on the annealing results, we first test the proposed metallic sealing at room temperature. As Figure 4a shows, the seal formed at room temperature under a small pressure of 9.0 MPa 1/2 1.3 MPa for five minutes consists of continuous solid regions; a longer compression time of 30 minutes leads to visually the same seal. Details of the sealing process are available in Supplemental Materials section S4. Although voids exist, the two substrates are well connected, leaving no apparent gap. The absence of gaps will provide the leak resistance, as our measurements of air leak rate will confirm later. In contrast, earlier attempts using Cu nanorods resulted in metallic seals with an apparent gap between the two substrates, even at much higher sealing temperatures of 200uC and 300uC17. To test the effects of faster surface diffusion, we have repeated the sealing process at 100uC 1/2 8uC for five minutes. As shown in Figure 4b, sealing at 100uC essentially eliminates voids beyond the size of a few nanometers. Going beyond the morphologies of the seals, we now put the seal of Figure 4a to the test for air leak; see section S4 of the Supplemental Materials for details of the setup and measurements. According to direct measurement of pressure degradation as a function of time inside a sealed vacuum, we determine the air leak rate to be less than 6.7 3 10210 cm3atm/s, taking into account a very conservative error bar. To appreciate how small this leak rate is, we compare it with (1) the leak rate of polymeric adhesive, and (2) the desired standards of the OSC and OLED industries. First, repeating the leak test with polymeric glue, we determine the leak rate to be at least 1000 times higher than that of the metallic seal. Second, when it comes to the industry standard, the requirements of leak resistance are 1 3 1023 cm3atm/m2/day for O2 to 1 3 1024 cm3atm/m2/day for H2O vapor, for a reference configuration of 1 m 3 1 m square solar
Figure 2 | Schematic of metallic nanorod sealing. Schematics of metallic nanorods (gray) on metallic film (gray) and substrate (dark), (a) before, (b) during, and (c) after the sealing process. SCIENTIFIC REPORTS | 3 : 3066 | DOI: 10.1038/srep03066
Figure 3 | Ag nanorod annealing. SEM images of Ag nanorods (a) before annealing from a top view, with 2u imaging titled cross-section view as inset; and after annealing for five minutes at (b) 50uC, (c) 75uC, and (d) 100uC. The scale bars in cross-sectional images are 100 nm.
panel1. For such a reference configuration, the air leak rate of our metallic seal is equivalently 1.5 3 1023 cm3atm/m2/day. Considering that 21% of typical air is O2 and 3% is H2O vapor (in volume), the corresponding leak rate of O2 is 3.2 3 1024 cm3 atm/m2/day and that of H2O vapor is 4.5 3 1025 cm3 atm/m2/day20. These are several times better than the industry requirements for both O2 and H2O vapor1. We note that this seal of better-than-required leak rate is achieved at room temperature under small mechanical pressure of 9.0 MPa, and also in ambient environment. Since the seal from room temperature processing suffices, here we will not pursue the test of seals from higher temperature processing. As an additional step, we have examined the mechanical shear strength of the metallic seal. Using lap shear pull tests, we determine the lower limit of the shear strength of the seal in Figure 4a to be 8.9 MPa; see Supplemental S5 for details of measurements. Repeating the tests using seals formed under mechanical pressure of about 5 MPa, we find that the air leak rate does not change by more than 10% but mechanical delamination occurs between the seal and the polymeric substrates. That is, for both air leak resistance and mechanical strength, the mechanical compression of up to about 10 MPa is appropriate.
Discussion In passing, we note that the spacing between nanorods is an important factor in the performance of the seal. In previous attempts, Cu nanorods are close to each other with small spacing17. The small spacing does not accommodate interpenetration of nanorods that are shown in Figure 2b, and therefore does not facilitate interlinking. As a result, two separate films formed under annealing without sufficient diffusion between the respective nanorod layers from each substrate. Here, the nanorods are spaced sufficiently far apart so that interpenetration occurs when two substrates are placed facing one another. That is, sufficient spacing between nanorods to allow interpenetration and crosslinking is critical to the sealing process. In summary, we report a metallic sealing process at room temperature under small mechanical pressure of 9.0 MPa, and also in ambient environment, for the first time. Through the easily accessible process, the resulting metallic seal has an air leak rate that is 1000 times better than that of polymeric glue, and several times better than that desired by the OSC and OLED industries1. Multiple technologies – such as OSCs and OLEDs – will benefit from this metallic sealing process.
Figure 4 | Seal morphologies. Cross-sectional SEM images of seals between two substrates under a small mechanical pressure of 9.0 MPa in ambient for five minutes (a) at room temperature, and (b) at 100uC. SCIENTIFIC REPORTS | 3 : 3066 | DOI: 10.1038/srep03066
www.nature.com/scientificreports 1. Krebs, F. C. & Norrman, K. Analysis of the failure mechanism for a stable organic photovoltaic during 10,000 h of testing. Prog. Photovoltaics Res. Appl. 15, 697–712 (2007). 2. Forrest, S. R. The path to ubiquitous and low-cost organic electronic appliances on plastic. Nature 428, 911–918 (2004). 3. Kawano, K. et al. Degradation of organic solar cells due to air exposure. Solar Energy Mater. Solar Cells 90, 3520–3530 (2006). 4. Dennler, G. et al. A new encapsulation solution for flexible organic solar cells. Thin Solid Films 511, 349–353 (2006). 5. Burrows, P. et al. Reliability and degradation of organic light emitting devices. Appl. Phys. Lett. 65, 2922–2924 (1994). 6. Lewis, J. Material challenge for flexible organic devices. Mater. Today 9, 38–45 (2006). 7. Reineke, S. et al. White organic light-emitting diodes with fluorescent tube efficiency. Nature 459, 234–238 (2009). 8. Niu, X. B., Stagon, S. P., Huang, H. C., Baldwin, J. K. & Misra, A. Smallest metallic nanorods using physical vapor deposition. Phys. Rev. Lett. 110, 136102 (2013). 9. Ma, H. & Suhling, J. C. A review of mechanical properties of lead-free solders for electronic packaging. J. Mater. Sci. 44, 1141–1158 (2009). 10. Rathmell, A. R., Bergin, S. M., Hua, Y., Li, Z. & Wiley, B. J. The growth mechanism of copper nanowires and their properties in flexible, transparent conducting films. Adv. Mater 22, 3558–3563 (2010). 11. Abtew, M. & Selvaduray, G. Lead-free solders in microelectronics. Mat. Sci. Eng., R 27, 95–141 (2000). 12. Akande, W. O., Cao, Y., Yao, N. & Soboyejo, W. Adhesion and the cold welding of gold-silver thin films. J. Appl. Phys. 107, 043519 (2010). 13. Abu-Isa, I. A., Jaynes, C. B. & O’Gara, J. F. High-impact-strength poly (ethylene terephthalate)(PET) from virgin and recycled resins. J. Appl. Polym. Sci. 59, 1957–1971 (1996). 14. Lu, Y., Huang, J. Y., Wang, C., Sun, S. & Lou, J. Cold welding of ultrathin gold nanowires. Nat. Nanotechnol. 5, 218–224 (2010). 15. Alarifi, H., Hu, A., Yavuz, M. & Zhou, Y. N. Silver nanoparticle paste for lowtemperature bonding of copper. J. Electron Mater. 40, 1394–1402 (2011). 16. Magdassi, S., Grouchko, M., Berezin, O. & Kamyshny, A. Triggering the sintering of silver nanoparticles at room temperature. ACS Nano 4, 1943–1948 (2010).
SCIENTIFIC REPORTS | 3 : 3066 | DOI: 10.1038/srep03066
17. Wang, P. et al. Low temperature wafer bonding by copper nanorod array. Electrochem. Solid-State Lett. 12, H138–H141 (2009). 18. Huang, H. C. A framework of growing crystalline nanorods. JOM 64, 1253 (2012). 19. Green, M. A. Estimates of Te and In prices from direct mining of known ores. Prog. Photovolt: Res. Appl. 17, 347–359 (2009). 20. Brimblecombe, P. [The atmosphere] Air composition and chemistry 1–19 (Cambridge University Press, New York, 1996).
Acknowledgements The authors acknowledge the financial support of US DoE Office of Basic Energy Science (DE-FG02-09ER46562). They also thank Roger Ristau for assistance in FIB milling experiments, and Paul Elliott for assistance in PVD experiments.
Author contributions H.H. and S.S. designed the project, analyzed the results, and wrote the manuscript together; and S.S. performed the experiments.
Additional information Supplementary information accompanies this paper at http://www.nature.com/ scientificreports Competing financial interests: The authors declare no competing financial interests. How to cite this article: Stagon, S.P. & Huang, H. Airtight metallic sealing at room temperature under small mechanical pressure. Sci. Rep. 3, 3066; DOI:10.1038/srep03066 (2013). This work is licensed under a Creative Commons AttributionNonCommercial-NoDerivs 3.0 Unported license. To view a copy of this license, visit http://creativecommons.org/licenses/by-nc-nd/3.0